# electronic and vibrational properties of monolayer

Embed Size (px)

TRANSCRIPT

Electronic and Vibrational Properties ofMonolayer Hexagonal Indium Chalcogenides

V. Zolyomi, N. D. Drummond and V. I. Fal’ko

Department of Physics, Lancaster University

QMC in the Apuan Alps IX, TTI, Tuscany, Italy

Friday 1st August, 2014

Introduction: Gallium and Indium Chalcogenides

• Two-dimensional materials: graphene, hexagonal boron nitride, silicene, germanane,a variety of transition metal dichalcogenides, gallium chalcogenides, . . .

• New members of the family: gallium chalcogenides (Ga2S2, Ga2Se2 and Ga2Te2)and indium chalcogenides (In2X2, In2Se2 and In2Te2). We will focus on the latter.

• Indium chalcogenides take a wide variety of forms, including tetragonal, rhombohedral,cubic, monoclinic, orthorhombic and hexagonal phases.

• Indium selenide (InSe) exists in a layered hexagonal structure in nature with anin-plane lattice parameter of 4.05 A and vertical lattice parameter of 16.93 A.

– InSe has been proposed for use in ultrahigh-density electron-beam data storage.– Very recently, Ajayan and coworkers at Rice University and Los Alamos have

succeeded in producing samples of few-layer (4–11 layers) hexagonal InSe bymechanical exfoliation.

• Indium sulphide (InS) and indium telluride (InTe) exhibit orthorhombic and tetragonalstructures, respectively, but it may be possible to prepare a hexagonal structure.

Structure of α Indium Chalcogenides

• Structure of α-In2X2 monolayers:

– Viewed from above, the monolayer forms a 2D honeycomb lattice.– Vertically aligned In2 and X2 pairs at hexagonal A and B sublattice sites.– The In atoms in each In2 dimer are bound together, and each In atom is bound to

the neighbouring X atoms.– Distance between the atoms within each X2 pair is considerably larger.– D3h point group (includes z → −z reflectional symmetry).

Structure of β Indium Chalcogenides

• Structure of β-In2X2 monolayers:

– Vertically aligned In2 dimers are located at hexagonal A sublattice sites.– One layer of X atoms is located at the B sublattice sites.– The other layer of X atoms is located at the C sublattice sites.– D3d point group (includes inversion symmetry).

Computational Methodology and Structural Parameters

• Density functional theory using the CASTEP and VASP plane-wave-basis codes.

– LDA, PBE and HSE06 functionals (latter only for calculating the band structure).– Phonon dispersion curves calculated using both finite displacements and density

functional perturbation theory.

• Experimental lattice parameter of bulk hexagonal InSe: a = 4.05 A.

– C.f., for monolayer α-In2Se2, a = 3.95 and 4.09 A according to the LDA and PBEfunctionals, respectively.

– LDA bond lengths are systematically smaller than the PBE bond lengths.

• Lattice parameters increase with the atomic number of the chalcogen, while the In–Inbond lengths hardly change.

Cohesive (Atomisation) Energy

• Cohesive energy Ec: energy of two isolated indium atoms plus the energy of twoisolated chalcogen atoms minus the energy per unit cell of the In2X2 layer.

– Difference between LDA and PBE cohesive energies is significant; nevertheless,both predict the cohesive energy to be largest for In2S2 and smallest for In2Te2.

– The β structures are dynamically stable, but the static-lattice cohesive energy isslightly less than that of the α structures (by 0.022 and 0.013 eV per unit cellaccording to the LDA and PBE functionals, respectively).

– Very small energy difference between the structures.– Inclusion of phonon zero-point energy makes no difference to this conclusion.– There is almost certainly a significant energy barrier between the two structures.– Might find domains of the two structures in samples.

α-In2Se2 Phonon Dispersion Curve

0

50

100

150

200

250

Γ K M Γ

ω (

cm

-1)

In2Se2 DFPT LDAIn2Se2 DFPT PBE

β-In2Se2 Phonon Dispersion Curve

0

50

100

150

200

250

Γ K M Γ

ω (

cm

-1)

In2Se2 DFPT LDAIn2Se2 DFPT PBE

Lattice Dynamics

• We find no imaginary phonon frequencies, other than a small pocket near Γ.

– Small pocket of instability: ubiquitous problem in first-principles calculations for2D materials. Difficult to converge the flexural (ZA) branch.

– Isolated atomic crystals of hexagonal indium chalcogenides (both α and β phases)are dynamically stable.

• The nonanalytic contribution to the dynamical matrix due to long-range Coulombinteractions (longitudinal/transverse optic mode splitting) is neglected in this work.

• The PBE functional predicts softer phonons than the LDA.

• Infrared and Raman spectroscopy: zone-centre optic phonons allow experimentalclassification of these materials.

– A normal mode is infrared active if it affects the dipole moment.– A normal mode is Raman active if it affects the polarisability.

Analysis of Zone-Centre LDA Optical Phonons For α-In2X2

Γ-pt. freq. (cm−1) IR int. (D2A−2amu−1) RamanBranch

In2S2 In2Se2 In2Te2Irrep.

In2S2 In2Se2 In2Te2 activity

4 40.6 35.6 30.7 E′′ – – – Ez ↔ E‖5 40.6 35.6 30.7 E′′ – – – Ez ↔ E‖

6 135 107 85.4 A′1 – – –{

E‖↔E‖Ez↔Ez

7 262 178 146 E′′ – – – Ez ↔ E‖8 262 178 146 E′′ – – – Ez ↔ E‖9 (TO) 264 181 150 E′ 10.2 (E‖) 5.18 3.57 E‖ ↔ E‖10 (LO) 264 181 150 E′ 10.2 (E‖) 5.18 3.57 E‖ ↔ E‖11 (ZO) 282 199 162 A′′2 0.25 (Ez) 0.10 0.061 –

12 293 228 207 A′1 – – –{

E‖↔E‖Ez↔Ez

• Experimental resonant Raman frequencies of few-layer InSe: 115 cm−1 (A′1), 179cm−1 (E′′), 187 cm−1 (A′′2), 201 cm−1 (A′′2), 212 cm−1 (E′) and 227 cm−1 (A′1).

• Experimental non-resonant Raman frequencies of few-layer InSe: 117 cm−1 (A′1),179 cm−1 (E′′) and 227 cm−1 (A′1).

Analysis of Zone-Centre LDA Optical Phonons For β-In2X2

Γ-pt. freq. (cm−1) IR int. (D2A−2amu−1) RamanBranch

In2S2 In2Se2 In2Te2Irrep.

In2S2 In2Se2 In2Te2 activity

4 40.8 35.8 31.2 Eg – – –

{E‖↔E‖E‖↔Ez

5 40.8 35.8 31.2 Eg – – –

{E‖↔E‖E‖↔Ez

6 134 106 84.9 A1g – – –{

E‖↔E‖Ez↔Ez

7 261 177 146 Eg – – –

{E‖↔E‖E‖↔Ez

8 261 177 146 Eg – – –

{E‖↔E‖E‖↔Ez

9 (TO) 262 180 149 Eu 10.4 (E‖) 5.4 3.8 –

10 (LO) 262 180 149 Eu 10.4 (E‖) 5.4 3.8 –

11 (ZO) 281 198 161 A2u 0.25 (Ez) 0.10 0.06 –

12 293 228 207 A1g – – –{

E‖↔E‖Ez↔Ez

• The frequencies are very similar in the two polytypes.

• Two modes are Raman-active in the α structure but not the β structure: means ofdistinguishing the phases.

α-In2Se2 Band Structure

-4

-3

-2

-1

0

1

2

3

4

Γ K M Γ

Energ

y -

EF (

eV

)

In2Se2 HSE06In2Se2 LDAIn2Se2 PBE

−0.4 −0.2 0 0.2 0.4−0.4

−0.2

0

0.2

0.4

kx (Å−1)

ky (Å−1)

−0.4 −0.2 0 0.2 0.4−0.4

−0.2

0

0.2

0.4

kx (Å−1)

ky (Å−1)

−0.4 −0.2 0 0.2 0.4−0.4

−0.2

0

0.2

0.4

In2Se2

kx (Å−1)

ky (Å−1)

• The LDA bands around the Fermi level are dominated by s- and p-type orbitals.

• Interband absorption selection rules:

– Photons polarised in-plane are absorbed by transitions between bands whose wavefunctions have the same z → −z symmetry (even→even and odd→odd);

– Photons polarised along the z axis cause transitions between bands with oppositesymmetry (even→odd and odd→even).

In2X2 Electronic Band Structures

• In2S2, In2Se2 and In2Te2: indirect-gap semiconductors, with the valence-bandmaximum (VBM) lying between Γ and K.

• The valence band has a saddle point on the Γ–M line.

– Lifshitz transition: when the hole concentration reaches the critical value where allstates are empty above the saddle point, the Fermi-surface topology changes.

– Carrier density at which Lifshitz transition takes place was found by integrating theDFT density of states from the saddle point to the valence-band edge.

• Valence band near VBM can be fitted by an inverted-Mexican-hat-shaped polynomial

EVB(k) =

3∑i=0

a2ik2i + a′6k

6 cos(6φ),

where φ is measured from the Γ–K line.

α-In2X2 Band Gaps, Spin-Splitting and Effective Masses (I)

Gap |∆EKSO| (meV) Elec. eff. mass m∗/me nLifshitz

(eV) VB CB Γc Kc Mc→Γc Mc

→Kc (1013 cm−2)α-In2S2 2.53 18 79 0.26 0.86 1.24 0.42 8.32α-In2Se2 2.16 92 23 0.20 0.71 2.30 0.33 6.00α-In2Te2 2.00 13 47 0.17 0.53 0.64 0.23 8.14

• The conduction-band minimum (CBM) is at the Γ point in all cases except the LDAband structure of α-In2Te2, where it is at the M point.

• There are local minima of the conduction band at Γ, K and M in each case, with theexception of the PBE band structure of α-In2Te2.

• Experimental gap of few-layer InSe (from photoconductivity spectra): 1.4 eV.

– Not much higher than the measured gap of bulk InSe (1.2 eV).– Differs from GaX, where the gap increases significantly in few-layer samples.– Lower than monolayer DFT-LDA gap (1.68 eV)!– Possibilities: difference between few-layer and monolayer In2X2 gaps; large excitonic

effects; few-layered sample contained a different structure.

α-In2X2 and β-In2X2 Electronic Band Structures

• β-In2X2 is also an indirect gapsemiconductor.

– The valence band is inverted-Mexican-hat-shaped around Γ,with the maximum on the Γ–Kline and a saddle point on the Γ–M line.

– The conduction band minimum isat Γ.

– Behaviour of conduction band atK and M is different, however.

Γ K M Γ

-4

-2

0

2

4

ε(k)

- ε F

(eV

)

α-In2Se

2

β-In2Se

2

• β-In2X2 gaps are smaller than α-In2X2 gaps by about 0.1 eV.

• Some of the bands exhibit spin splitting, including the highest valence (∆Ev,KSO ) and

lowest conduction (∆Ec,KSO ) bands near the K point.

In2Se2 Optical Absorption Spectra

0

5

10

0 2 4 6 8 10 12 14 0

10

20

30

Absorp

tion c

oeffic

ient (%

)

Im (

ε)

Energy (eV)

α-In2Se2 LDA, in-planeα-In2Se2 LDA, out-of-plane

β-In2Se2 LDA, in-planeβ-In2Se2 LDA, out-of-plane

• Absorption shows a prominent peak (originating from the vicinity of the K point) at3–5 eV, where the absorption coefficient of In2Se2 is similar to that of graphene.

– Ultrathin films of InX biased in vertical tunnelling transistors with grapheneelectrodes could be used as an active element for the detection of UV photons.

Conclusions

• DFT indicates that the 2D hexagonal indium chalcogenides In2S2, In2Se2 and In2Te2

are dynamically stable, indirect-band-gap semiconductors with an unusual inverted-Mexican-hat-shaped valence band.

• We have provided the phonon frequencies and Raman and IR activities of modes, toassist the identification of these structures.

• Two possible structures (α and β) were investigated, which are very close in energy.

• Saddle points in the valence band along the Γ–M line lead to a Lifshitz transition inthe event of hole doping, for which we have calculated the critical carrier density.

• We have given a qualitative description of the optical absorption spectra, whichsuggest that atomically thin films of indium chalcogenides could find application inultraviolet photon detectors.

To-Do (Where QMC Finally Gets a Mention)

• Study bulk InX and GaX, to understand stacking effects in the multilayer samplesthat experimentalists are currently actually working with.

– Two polytypes for each layer: α and β. Can invert/reflect these to give α′ and β′.– Two stacking arrangements for In2 or Ga2 dimers: AA and AB.– The five AA-stacked structures: αα, αα′, αβ, ββ and ββ′.– The six AB-stacked structures: αα, αα′, αβ, α′β, ββ and ββ′.– Different exchange–correlation functionals and dispersion-correction schemes give

different relative energies on an energy scale of more than ∼ 0.02 eV per cell.– Use QMC to identify the most stable structures.– Problem: the In and Ga pseudopotentials from the CASINO library don’t work

at all in CASTEP and hence CASINO. Ghost states due to Kleinman–Bylanderrepresentation? Use DFT pseudopotentials?

– Determine the Raman/IR-active phonon modes to help the experimentalists.

• Use DMC to investigate the quasiparticle gaps and exciton binding energies.

– DMC and GW0 studies of hexagonal BN indicate that the latter underestimatesthe quasiparticle gap by more than 1.5 eV (and G0W0 is even worse).

Acknowledgements

• We acknowledge financial support from EC-FET European Graphene Flagship Project,EPSRC Science and Innovation Award, ERC Synergy Grant “Hetero2D”, the RoyalSociety Wolfson Merit Award and the Marie Curie project CARBOTRON.

• Computational resources were provided by Lancaster University’s High-End Computingfacility.

• This work made use of the facilities of N8 HPC provided and funded by the N8consortium and EPSRC (Grant No. EP/K000225/1). The Centre is coordinated bythe Universities of Leeds and Manchester.